Hazardous plastic waste management and fuel production by
Hazardous Plastic Waste Management and FuelProduction by Pyrolysis -Harsh Bhatt
Sources of Plastic Waste:• Plastic waste can be mainly classified as:(1) Municipal Waste(2) Industrial Waste• Plastic wastes represent a considerable part of municipal wastes, while huge amounts of plastic waste arise as a by-product or faulty product in industry and agriculture• Of the total plastic waste, over 78 wt% of this total corresponds to thermoplastics and the remaining to thermosets
Sources of Plastic Waste• Thermoplastics are composed of polyolefins such as polyethylene, polypropylene, polystyrene and polyvinyl chloride and can be recycled• Thermosets mainly include epoxy resins and polyurethanes and cannot be recycled!• Determination of the Type of the waste and the appropriate method of its disposal is the heart of the entire process, and should be carried out with utmost care
Municipal Solid Waste• Municipal Solid Wastes (MSW) normally remain a part of municipal solid wastes as they are discarded and collected as household wastes• The various sources of MSW plastics includes(1)Domestic Waste (food containers, packaging foam, disposable cups, plates, cutlery, CD and cassette boxes. fridge liners, vending cups, electronic equipment cases, drainage pipe, carbonated drinks bottles, plumbing pipes and guttering, flooring. cushioning foams, thermal insulation foams, surface coatings, etc.)
Municipal Solid Waste(2) Municipal Waste (mulch films, feed bags, fertilizer bags, and in temporary tarpaulin-like uses such as covers for hay, silage, etc.)(3) Wires and Cables(4) Automobile Wrecking, etc.• Thus, the MSW collected plastics waste is mixed one with major components of polyethylene, polypropylene, polystyrene, polyvinyl chloride, polyethylene terephthalate, etc.
Industrial Plastic Waste• Industrial plastic wastes (so-called primary Waste) are those arising from the large plastics manufacturing, processing and packaging industry• The industrial waste plastic mainly constitute plastics from(1) Construction and Demolition companies (e.g. polyvinyl chloride pipes and fittings, tiles and sheets)(2) Electrical and Electronic Industries
Industrial Plastic Waste(e.g. switch boxes, cable sheaths, cassette boxes, TV screens, etc.)(3) The automotive industries spare-parts for cars (such as fan blades, seat coverings, battery containers and front grills)• Most of the industrial plastic waste have relatively good physical characteristics i.e. they are sufficiently clean and free of contamination and are available in fairly large quantities
Different Methods of Plastic Waste Management• Due to population increase, the demand for plastic products has steadily increased over the last few decades• Since plastics are nonbiodegradable, they cannot be easily returned to the natural carbon cycle; hence the life cycle of plastic materials ends at waste disposal facilities• There are several methods for disposal of municipal and industrial plastic waste, i.e. landfill, incineration (energy recovery), true material recycling (monomer recovery), and chemical recovery
Land-filling• Highest portion of the solid waste including plastics have been subjected to landfill• However, disposing of the waste to landfill is becoming undesirable due to(1) Legislative pressures (where waste to landfill must be reduced by 35% by 2020)(2) Rising costs
Land-filling(3)The generation of explosive greenhouse gases (such as methane)(4) The poor biodegradability of commonly used packaging polymers• In light of these hazards, the improvement in federal regulations for land filling are carried out by normalizing the use of liners in the landfill bed, ground water testing for waste leaks, and post landfill closure care• However, since waste plastics have a high volume to weight ratio, appropriate landfill space is becoming both scare and expensive
Mechanical Recycling• Mechanical recycling is reprocessing of the used plastics to form new similar products• This is a type of primary and secondary recycling of plastic where the homogeneous waste plastics are converted into products with nearly same or less performance level than the original product
Mechanical Recycling• Many efforts are made by the technologists to recover materials from waste plastics suitable for second use• Practical experience has shown that reprocessing of mixed contaminated plastics produces polymer polyblends that are inferior mechanically and lacking in durability (which is explained due to peroxidation) compared with those produced from virgin polymers• Although at first sight mechanical recycling of plastic wastes appears to be a ‘green’ operation, the re- processing operation is not cost effective
Mechanical Recycling• The reason for this process being non- costeffective includes(1) High energy required for cleaning, sorting, transportation and processing(2) The cost of additives used to provide a serviceable product can not be neglected• Again, materials recycling of household waste plastics is particularly difficult when they are contaminated with biological residues or, as is usually the case, when they are a mixture of different kinds of Plastics
Thermal Recycling (Incineration)• Energy generation by incineration of plastics waste is in principle a viable use for recovered waste polymers since hydrocarbon polymers replace fossil fuels and thus reduce the CO2 burden on the environment• Incineration is the preferred energy recovery option of local authorities because there is financial gain by selling waste plastics as fuel• The high caloric value of plastics can enhance the heating value of MSW and facilitate an efficient incineration, while their energy content can also be recovered.
Thermal Recycling (Incineration)• In most developed countries public distrust of incineration at present limits the potential of waste-to- energy technologies as it produce greenhouse gases and some highly toxic pollutants such as polychlorinated dibenzo para dioxins (PCDD) and polychlorinated dibenzo furans (PCDF)• The potential relationship between plastics fed into an incinerator and the formation of dioxins and furans is still unclear and has been suggested that the chlorine content in PVC and other plastics is related to the formation of dioxins and furans
Biological Recycling• Intensive research by Industries and Universities has led to the development of polymeric materials that conform to user requirements but are also returned to the biological cycle after use• This resulted in development of biodegradable polymers which can be converted back to the biomass in a realistic time period• They are introduced in food/catering industry which photo-degrades in six weeks, and in non- packaging applications such as computer or car components.
Biological Recycling• There are a number of concerns over the use of degradable plastics1. These plastics will only degrade if disposed of in appropriate conditions2. They may cause an increase in emissions of the greenhouse gas methane, as methane is released when materials biodegrade anaerobically3. The mixture of degradable and non-degradable plastics may complicate plastics sorting systems.
Biological Recycling4. The use of these materials may lead to an increase in plastics waste and litter if people believe that discarded plastics will simply disappear• Due to all these problems at present the biodegraded plastics cannot substitute all the application areas of synthetic plastics.
Chemical Recycling• Current state of the art Feedstock recycling, also known as chemical recycling or tertiary recycling, aims to convert waste polymer into original monomers or other valuable chemicals• These products are useful as feedstock for a variety of downstream industrial processes or as transportation fuels• There are three main approaches: depolymerisation, partial oxidation and cracking (thermal, catalytic and hydro cracking)
Depolymerization• Condensation polymers which include materials such as polyamides, polyesters, nylons and polyethylene terephthalate can be depolymerised via reversible synthesis reactions to initial diacids and diols or diamines• Typical depolymerisation reactions such as alcoholysis, glycolysis and hydrolysis yield high conversion to their raw monomers• Addition polymers which include materials such as polyolefins, typically making up 60– 70% of municipal solid waste plastics, cannot be easily depolymerised into the original monomers by reverse synthesis reaction.
Partial Oxidation• The direct combustion of polymer waste, which has a good calorific value, may be detrimental to the environment because of the production of noxious substances such as light hydrocarbons, NOx, sulfur oxides and dioxins• Partial oxidation (using oxygen and/or steam), however, could generate a mixture of hydrocarbons and synthesis gas (CO andH2), the quantity and quality being dependent on the type of polymer used.
Cracking (Pyrolysis)• As discussed earlier , Cracking Phenomena can be classified into 1. Hydro-cracking 2. Thermal-cracking 3. Catalytic-cracking
Hydro-cracking• Hydrocracking of polymer waste typically involves reaction with hydrogen over a catalyst in a stirred batch autoclave at moderate temperatures and pressures (typically 423–673 K and 3–10 MPa hydrogen)• This obtains a high quality gasoline starting from a wide range of feeds, that include polyethylene, polyethylene terephthalate, polystyrene, polyvinyl chloride and mixed polymers, polymer waste from municipal solid waste and other sources• Several catalysts, classically used in refinery hydrocracking reactions, have been evaluated and include transition metals (e.g., Pt, Ni, Mo, Fe) supported on acid solids (such as alumina, amorphous silica–alumina, zeolites and sulphated zirconia)
Thermal Cracking• Thermal cracking, involves the degradation of the polymeric materials by heating in the absence of oxygen• The process is usually conducted at temperatures between 350 and 900 8C and results in the formation of a carbonized char (solid residues) and a volatile fraction that may be separated into condensable hydrocarbon oil consisting of paraffins, isoparaffins, olefins, naphthenes and aromatics, and a noncondensable high calorific value gas• The thermal degradation of polymers to low molecular weight materials requires high temperatures and has a major drawback in that a very broad product range is
Catalytic Cracking• In this method a suitable catalyst is used to carry out the cracking reaction that lowers the reaction temperature and time• Catalytic degradation yields a much narrower product distribution of carbon atom number with a peak at lighter hydrocarbons and occurs at considerably lower temperatures• This method seem to be the most promising to be developed into a cost-effective commercial polymer recycling process to solve the acute environmental problem of plastic waste disposal
Pyrolysis of plastic waste to liquid fuel—the process• Pyrolysis is generally defined as the controlled burning or heating of a material in the absence of oxygen• In plastics pyrolysis, the macromolecular structures of polymers are broken down into smaller molecules or oligomers and sometimes monomeric units• Further degradation of these subsequent molecules depends on a number of different conditions including (and not limited to) temperature, residence time, and the presence of catalysts and other process conditions• The pyrolysis reaction can be carried out with or without the presence of catalyst, accordingly, the reaction will be thermal and catalytic pyrolysis
Thermal Pyrolysis of Plastic• The non-catalytic or thermal pyrolysis of polyolefins is a high energy, endothermic process requiring temperatures of at least 350–500 C, in some studies, temperatures as high as 700–900 C are essential in achieving decent product yields• Thermal cracking results in liquids with low octane value and higher residue contents at moderate temperatures, thus an inefficient process for producing gasoline range fuels
Thermal Pyrolysis of Plastic• The gaseous products obtained by thermal pyrolysis are not suitable for use as fuel products, requiring further refining to be upgraded to useable fuel products• A few researchers have sought to improve thermal pyrolysis of waste polyolefins without employing the use of catalysts; however these changes either yielded insignificant improvements or added another level of complexity and costs to the system• Many process have been devised and set-up to serve the conversion of Plastic waste to useful oil,but the first one to do this was ‘the Blest Corporation’ from Japan
Catalytic cracking of Plastics• Addition of catalyst enhances the conversion and fuel quality, as compared to the purely thermal pyrolysis, the addition of catalyst in polyolefin pyrolysis• The dramatic effect of catalyzed decomposition of polymers has spurred a wave of research in the area of catalysis and polymer degradation. And thus, Catalytic degradation of plastics is found to have greatest potential to be developed into a commercialized process
Comparison of waste plastics fuel to regular gasolineProperties Regular gasoline Plastic waste fuelColour, visual Orange Pale YellowSpecific gravity at 28 C 0.7423 0.7254Specific gravity at 15 C 0.7528 0.7365Gross calorific value 11210 11262Net calorific value 10460 10498API gravity 56.46 60.65Sulphur content(by mass) 0.1 <0.002Flash point (C) 23 22
Effect type of polymer on product yield and distribution• The primary pyrolysis products relates directly to the chemical structure and decomposition of the resin, and also to the mechanism of its decomposition• Waste polyolefins may degrade at slightly lower temperatures and achieve higher conversions than the respective virgin polyolefins• Pyrolysis of plastics yields liquid, gas and solid residue products. Liquid product yields greater than 82.5% and as high as 96% have been found for polyethylene and polypropylene pyrolysis , at high temperatures and within a reaction time of approximately one hour
Effect of catalyst loading• The use of catalyst in pyrolysis of plastics influences upon kinetics and mechanism, and hence, the product distribution hence, conversion increases with catalyst loading• The most commonly researched solid acid catalysts in plastic wastepyrolysis include molecular sieves, such as silica, alumina, zeolites and MCM-41• Amongst the numerous kinds of zeolites investigated in polyolefin pyrolysis, Beta , USY, ZSM-11, REY , Mordenite , ZSM-5 are the most commonly used• Other catalytic materials such as clays (montmorillonite, saponite), reforming catalysts, activated carbon, metal oxides, metal complexes of the type MCln–AlCl3 or M(AlCl4)n (M = Li, Na, K, Mg, Ca, Ba; n = 1–2), and alkali metal carbonates or alkaline metal carbonates have also been tested for polymer degradation
Process• The Process steps:1. Introduction of Plastic waste to the reactor2. Closing the lid of the reactor (air-tight) and apply heating3. Increase the heating gradually taking care that sudden temperature rise may not burn certain waste4. Collect the generated fumes on water
Apparatus required for the Process1. Reactor (with Lid)- keeping in mind the type of waste used2. Heater with precisely controlled step increase that gives temperature atleast upto 500 C3. A transparent vessel that will collect extracted oil on water and should have a tap to collect Oil when cycle is over4. Off-gas Filter5. Fractional distillation of oil to kerosene, diesel and gasoline
Off-gas Filter• Some gases that will be generated during the Process cannot be liquified that include Butane, ethene, methane etc.• If this gases are liberated to atmosphere , they will have toxic effects in atmosphere and also cause harm to workers/operators in contact with machinery in long run• This gase are hence converted to harmless components like Carbon dioxide and water with the use of the off-gas filter
Process Design• Many have demonstrated that plastics waste can indeed be converted to useful chemical feedstock by both non-catalytic and catalytic pyrolysis• The distribution can also be affected by different process parameters such as feed composition (plastic type), catalyst loading, size of the catalyst, the means of polymer and catalyst contact during degradation, reactor type, and degradation process conditions such as temperature, pressure, residence time• The effect of various process variables are as follows